chapter 2 hyperbranched polymers via acyclic a simple method for the preparation of hyperbranched...
Post on 27-Apr-2018
Embed Size (px)
Hyperbranched Polymers via Acyclic Diene Metathesis Polymerization
Portions of this chapter have previously appeared as: Gorodetskaya, I. A.; Choi, T. L.;
Grubbs, R. H. J. Am. Chem. Soc. 2007, 129, 12672-12673.
A facile route to hyperbranched polymers via acyclic diene metathesis is described.
According to this new methodology, a variety of molecules functionalized with two or
more acrylate groups and one terminal aliphatic alkene can serve as an ABn monomer when
exposed to an imidazolinylidene-based ruthenium olefin metathesis catalyst, due to the
cross metathesis selectivity of this catalyst. For the polymers obtained by this method, both
1H NMR spectroscopy and triple detector size exclusion chromatography conclusively
indicate a branched architecture.
Hyperbranched polymers are highly branched macromolecules typically prepared
via a one-pot polymerization of ABn2 monomers (Scheme 2.1A).1-6 The A and B
functionalities of these monomers readily react with each other (A reacts with B and vice
versa) but not with themselves (A does not react with A and B does not react with B). The
approach to the preparation of hyperbranched polymers was originally described by Flory
as early as 1952, but, at the time, such an architecture was mainly of theoretical interest.7
However, it has since been discovered that the unique macromolecular architecture of these
polymers gives rise to many attractive, practical features such as multiple end groups,
improved solubility, and lower solution viscosity (relative to linear analogues of the same
molecular weight).1-6 Moreover, dendrimers
8-10structurally perfect, monodisperse
hyperbranched macromoleculeshave already found applications in medicine,11,12
Unfortunately, dendrimer iterative synthesis and
purification can be rather labor-intensive and, thus, expensive (Scheme 2.1B).8-10 As such,
the preparation and study of hyperbranched polymers, which typically exhibit properties
similar to those of monodisperse dendrimers,17,18
have been extensively pursued in recent
Scheme 2.1. Synthesis of dendritic polymers.
In the 55 years since Florys theoretical report, as interest in dendrimers and
hyperbranched polymers increased, a large number of synthetic approaches to these
macromolecules have been reported. Moreover, the range of methods available for
hyperbranched synthesis has expanded well beyond classical step-growth condensations
and additions of AB2 monomers6 to include such notable examples as self-condensing vinyl
polymerization (SCVP) of AB* monomers,19 various ring-opening polymerizations of
latent ABn monomers,20-22
and proton-transfer polymerization.23 However, many of these
methods have significant drawbacks such as harsh reaction conditions and the need for
complex monomers. Although olefin metathesis has never previously been used to prepare
hyperbranched architectures, it is well-suited for the task because it requires very mild
reaction conditions and possesses good functional group tolerance, which allows access to
a great variety of polymer backbones from readily available monomers. This chapter
describes a simple method for the preparation of hyperbranched polymers via acyclic diene
metathesis polymerization (ADMET).24
Results and Discussion
Catalyst 1 (Figure 2.1) was selected for the ADMET hyperbranched
polymerization. This imidazolinylidene-based catalyst is tolerant of many functional
groups, stable to air and moisture, and readily promotes cross metathesis between electron-
rich primary olefins. Furthermore, it can catalyze cross metathesis involving low
metathesis-reactive olefins, such as electron-deficient alkenes. When treated with 1,
electron-poor olefins do not homodimerize (or do so very slowly), but do participate in a
secondary metathesis reaction with homodimers of more reactive olefins.25 Therefore, a
molecule functionalized with one electron-rich olefin, such as a terminal alkene, and two or
more electron-poor olefins, such as acrylates, is an ABn-type monomer (Figure 2.2) that
can be polymerized into a hyperbranched structure using catalyst 1 (Scheme 2.2). In fact, a
similar concept has been previously demonstrated in the synthesis of alternating
copolymers26 and various small molecules.
Figure 2.1. Acyclic diene metathesis polymerization catalyst.
Figure 2.2. Monomers for hyperbranched ADMET polymerization
Scheme 2.2. Synthesis of AB2 monomer 4 and its hyperbranched ADMET polymerization.
Monomers 27 (Figure 2.2) were utilized for the ADMET hyperbranched
polymerization. They were prepared in one to four steps from commercially available,
inexpensive starting materials such as glycerol, pentaerythritol, and 5-hydroxyisophthalic
acid. 2 and 3 were prepared as linear analogues to AB2 monomers 4 and 5, as well as the
AB3 monomer 7. To further demonstrate the inherent flexibility of the presented method,
monomer 6 was also synthesized to make a hyperbranched polymer with a different
The polymerization of each monomer is easily monitored by 1H NMR
For example, Figure 2.3 shows the 1H NMR spectra of 4 and the
resulting crude polymer 4a. Some peak broadening due to formation of macromolecules
can be observed in the spectrum of 4a, especially for the backbone proton b. It can also be
seen that the terminal olefins (a) completely disappear during the polymerization.
Moreover, as expected, a new peak (g), a doublet of triplets, appears at 6.95 ppm due to
formation of internal acrylates (AB olefins). Furthermore, if polymerization proceeds to
completion, as is the case here, all of the terminal aliphatic alkenes are consumed and there
should be half of the free acrylate groups left in the final polymer. Since there are twice as
many B groups as A groups in an AB2 monomer, an integration ratio of 1 (g) to 1 (c or d)
should hold for the product of complete polymerization. Indeed, a 1:1 ratio is observed for
4a (Figure 2.3), as well as 5a and 6a; it is 2:1 for 7a. Peaks d, c, and e completely
disappear, along with the peaks for protons a, during the polymerizations of 2 and 3, and
the integration ratio of the corresponding polymer peaks g and f is 1:1.
Figure 2.3. 1H NMR spectra of monomer 4 (top) and hyperbranched polymer 4a (bottom).
A multiangle light-scattering (MALS) detector combined with a differential
refractometer and an on-line viscometer following size exclusion chromatography (SEC)
was used to determine the molecular weights and PDIs of the obtained polymers.
Additionally, viscometer data helped to characterize branching of the macromolecules
resulting from ADMET of 27. Table 2.1 summarizes the typical crude polymerization
results. The observed PDI values are quite high, which is typical for a hyperbranched step-
growth type polymerization.30
Table 2.1. Results of polymerization of 27.a
Polymer Mw (kDa) Mn (kDa) PDI x 10-1
2a 4.31 2.07 2.1 4.45 0.01
3a 21.43 4.44 4.8 4.12 0.02
4a 3.61 0.55 6.5 3.82 0.02
5a 14.77 3.08 4.8 3.24 0.02
6a 10.24 3.17 3.2 3.34 0.03
7a 30.90 5.00 6.2 2.69 0.02
a Polymerization conditions: 0.5 mol % of 1 was used and the polymerizations were conducted in near-
refluxing methylene chloride (43 oC) with venting. Mw, Mn, and PDI were calculated from triple-angle laser
light scattering and refractive index measurements. was measured with an on-line differential viscometer.
Figure 2.4 compares the plots of intrinsic viscosity (IV) vs. molecular weight
(MarkHouwinkSakurada plots) for polymers 2a7a. As expected, the IV of branched
polymers 4a7a is much lower than that of the linear polymer 2a for any given molecular
weight. Interestingly, the supposedly linear polymer 3a has a drastically reduced intrinsic
viscosity compared to that of 2a, although not quite as low as the viscosities of branched
polymers. This property of 3a can be attributed to the presence of a methoxy-methyl
pendant group in each monomer unit. This group is inert during the polymerization, but its
length is comparable to the monomers overall size. Such an architecture results in a
comb-type polymer with a lower than expected IV (relative to that of a linear
analogue).31 Across the molecular weight range studied, the viscosity of polymer 7a, based
on an AB3 monomer 7, is even lower than that of AB2 polymers 4a6a. This observation
indicates even more branching in the AB3-based polymer. On the other hand, the intrinsic
viscosity does not change dramatically with slight variations in the backbone; it can be seen
from Figure 2.4 that the MarkHouwink plots for 4a6a completely overlap.
Figure 2.4. Mark-Houwink-Sakurada plots for polymers 2a7a.
To extend the analysis, the MarkHouwink shape parameter ( = KM) for
polymers 2a7a were compared (Table 2.1). An parameter of 0.51.0 is typical for
randomly coiled linear polymers.32 Polymers with a rigid-rod shape have an of 2.0, and
spherically shaped m